ASTM Epdf – Download as PDF File .pdf), Text File .txt) or read online. ASTM E Standard Practice for Microetching Metals and Alloys. Basic Description: ASTM E is a method of etching a metal sample to reveal its microstructure. On a microscopic scale, metal is made up of many grains which.
|Published (Last):||3 December 2008|
|PDF File Size:||8.39 Mb|
|ePub File Size:||20.94 Mb|
|Price:||Free* [*Free Regsitration Required]|
Pure Th Th alloys Tin Base: Immerse until surface is colored. Swab until stain is removed. Where ethanol or methanol, or both are listed as alternates, ethanol is the preferred solvent.
ASTM E – 07()e1 Standard Practice for Microetching Metals and Alloys
Rinse in Solution B. Total etching time 3 min 50 mL Carbitol diethylene glycol monoethyl with agitation. Immerse to 1 min. Film on etched aluminum bronze removed by No. Swab 3—10 s or immerse to 2 min.
Electrolytic at 9—12 V for 1—10 min. Immerse or swab to 1 min. The specimen is examined as polished under polarized light. For highly corrosion-resistant alloys, use 20—30 mL HCl. Remove the specimen from the etchant when the surface is atsm violet, rinse and dry. A vacuum level of 1. Agitate solution gently until coloration begins, allow to settle.
For best results use before pellets r407 dissolved. Use a polyethylene beaker to contain the etchant if it contains? Additionally, one can contact the glove manufacturer or, if available, consult the manufacturers glove chart.
Standard Practice for Microetching Metals and Alloys
Can be heated to increase activity. Swab 2 or more minutes for desired surface. Polishes at high currents. Distilled water is then slowly added to the wheel and polishing continued until the surface is bright.
Immerse 10 min or longer. Use at 1 V dc, s, with stainless cathode; 0. Composition Electrolytic at 2—3 V for 2—10 s.
Immerse or swab few seconds to few minutes. Clean in HNO3 if necessary. Immerse to several minutes. Electrolytic at 6 V for 10—20 s. One or several small lumps of a suitable dielectric compound with the desired index of refraction is heated under a vacuum until it evaporates.
It will also react with alkaline materials including plaster and concrete to form explosive compounds. Add the HCl just before using.
Immerse specimen face up, gently agitate solution until coloration begins, allow to settle. Rinse with ethanol or methanol and blow dry. This standard asttm been approved for use by agencies of the Department of Defense.